Catalyst-Doped Anodic TiO 2 Nanotubes: Binder-Free Electrodes for (Photo)Electrochemical Reactions

: Nanotubes of the transition metal oxide, TiO 2 , prepared by electrochemical anodization have been investigated and utilized in many ﬁelds because of their speciﬁc physical and chemical properties. However, the usage of bare anodic TiO 2 nanotubes in (photo)electrochemical reactions is limited by their higher charge transfer resistance and higher bandgaps than those of semiconductor or metal catalysts. In this review, we describe several techniques for doping TiO 2 nanotubes with suitable catalysts or active materials to overcome the insulating properties of TiO 2 and enhance its charge transfer reaction, and we suggest anodization parameters for the formation of TiO 2 nanotubes. We then focus on the (photo)electrochemistry and photocatalysis-related applications of catalyst-doped anodic TiO 2 nanotubes grown on Ti foil, including water electrolysis, photocatalysis, and solar cells. We also discuss key examples of the effects of doping and the resulting improvements in the efﬁciency of doped TiO 2 electrodes for the desired (photo)electrochemical reactions. results measured for different nanotube materials in identical alkaline OER tests. Reproduced with permission [31]. Inha


Introduction
Anodization is a facile process that allows the physical and chemical properties of an entire metal surface to be modified at a very low cost, and it has long been recognized as a well-established industrial surface treatment technique [1,2]. In particular, the discovery of self-ordering phenomena in anodic aluminum oxide produced using two-step anodization [3][4][5][6] led to great advances in nanoscience applications based on highly ordered nanoporous Al 2 O 3 membranes and triggered the search for new alternative anodic materials with intrinsic semiconductive properties induced by external electrical or photo stimuli [7].
Since the formed oxide adheres to and remains in stable contact with the mother metal material without any binder, high-surface-area anodic titanium oxide has been considered for use as an electrode for (photo)electrochemical reactions in strong acidic or basic conditions [17,18]. In general, electrodes should require a low overpotential for initiating the targeted reaction in order to increase current efficiency. However, oxide-based electrodes containing anodic titanium oxide are disadvantageous the bottom of nanotubes grows significantly thicker with increasing potential shock voltage, blocking current flow. Although higher potentials produce higher doping concentrations in the nanotubes, very high potential shock voltages cannot be used due to the barrier layer growth. Therefore, optimization of the potential shock voltage always involves a trade-off between achieving a high degree of doping and reducing the growth of the barrier oxide. Additionally, although electrolytes with high precursor concentrations result in higher doping concentrations in TiO 2 , in some cases the target potential cannot be maintained due to the limiting current-compliance of the power supply [34]. Thus, low potential shock voltages and low concentrations of doping precursors are preferred in the potential shock method, meaning that relatively low doping concentrations are achieved. In general, Cl − -based ions destroy or break down nanotubular structures during simultaneous single-step anodization or potential shock doping. However, some novel metal precursors inherently produce Cl − ; for example, H 2 PtCl 6 is dissociated to 2H + + PtCl 6 2− , which generates Cl − ions. In such cases, underpotential shock, in which the potential shock voltage is lower than that used for anodization, has been successfully demonstrated as an alternative doping method. In that case, the Pt ions penetrate only the middle of the oxide layer where the low potential shock voltage has an influence, rather than reaching the interface of the barrier oxide and the Ti metal [33]. The anodization of alloys is another method to produce doped TiO 2 nanotubes; however, the alloying process is very elaborate compared to the fabrication of Ti metal alone. Due to limit of availability of Ti-based alloys and their cost, a great deal of work to develop easily reproducible metal alloys at low cost is still required [30]. Additionally, the inevitable thermal growth of additional oxides and crystal phase changes as a function of the temperature during the annealing process should be considered [35].
Recently, a number of review or prospective articles related to anodic TiO 2 and its applications have been published. For example, Lee et al. comprehensively reviewed one-dimensional titanium oxides grown by anodization [8]. More specifically, several groups have published reviews of photo-catalysis or electro-catalysis applications based on anodic TiO 2 [36][37][38][39][40]. Additionally, bio-related applications of anodic TiO 2 materials have also been reviewed recently [41,42].
In this review, we focus on the use of TiO 2 nanotubes as (photo)electrochemical binder-free electrodes in applications that require low overpotential or narrow bandgaps to achieve the desired reactions. Various doping processes to adjust the overpotential and bandgap are comprehensively reviewed.

Reaction Mechanism
The formation of TiO 2 nanotubes is governed by two competitive reactions: (1) oxide formation at the oxide/metal interface by oxygen anions (O 2 − and OH − ), and (2) the dissolution reaction caused by the F − in the electrolyte ( Figure 1) [2,8,10,11,16,36]. In oxide formation, O 2 − and OH − anions eVolve on the electrolyte/oxide interface via the electrolysis of water. These anions diffuse through the oxide layer to come into contact with the metal interface. Simultaneously, Ti 4+ moves through the oxide layer in the opposite direction, and reacts directly with oxygen anions. eVentually, TiO 2 is generated as shown in the equation below [8,11,16,43].
Ti + 2H 2 O → TiO 2 + 4H + + 4e − , In short, the oxide formation rate is governed by the diffusion and reaction rates of the oxygen anions in the oxide layer. The newly formed oxide pushes up the existing oxide and gradually grows toward the metal substrate. This phenomenon is known as "plastic flow" [11].  (d) and (e) the F − -rich layer is finally dissolved by the water in the electrolyte. Reproduced with permission from ref [11]. Friedrich-Alexander-Universität Erlangen-Nürnberg (2013).
Meanwhile, in the dissolution reaction, F − ions react with TiO2 directly at the electrolyte/oxide interface to produce [TiF6] 2− , which is easily dissolved into the electrolyte due to its high solubility in water. As the F − ions travel roughly twice as fast as the oxygen ions, they can contact and react directly with Ti 4+ at the oxide/metal interface. The relevant reaction equations are follows [8,11,16]: Due to the role of F − , the honeycomb-like porous structure transforms into an array of tubes with an F − -rich layer between the TiO2 layer and the Ti metal. As a result, a hemispherical oxide/metal interfacial structure is formed. The overall growth rate and the length of the nanotubes are determined by the difference between the oxide formation and dissolution reaction rates.
The current-time (I-t) behavior measured during the potentiostatic preparation of TiO2 nanotubes reflects this overall mechanism ( Figure 2). In the initial stage, the current decreases rapidly due to the increasing resistance of the rapidly growing oxide layer (I). In the second step (II), the current increases slightly due to the formation of nano-sized pits, which are formed due to attack by the F − ions. The local electric fields are strengthened in these pits, thus attracting more anions to participate in the oxide formation and dissolution reactions. As a tubular structure begins to form beneath the pits, the current decreases again (III). When the oxide formation and dissolution reactions reach equilibrium, the current converges (IV). The current-time transient itself cannot confirm the formation of nano-tubular structures, since non-nanotube-forming processes based on the barrier oxide formation, oxide pitting, and the stable growth mechanism show similar current patterns [11].  (d) and (e) the F − -rich layer is finally dissolved by the water in the electrolyte. Reproduced with permission from ref [11]. Friedrich-Alexander-Universität Erlangen-Nürnberg (2013).
Meanwhile, in the dissolution reaction, F − ions react with TiO 2 directly at the electrolyte/oxide interface to produce [TiF 6 ] 2− , which is easily dissolved into the electrolyte due to its high solubility in water. As the F − ions travel roughly twice as fast as the oxygen ions, they can contact and react directly with Ti 4+ at the oxide/metal interface. The relevant reaction equations are follows [8,11,16]: Due to the role of F − , the honeycomb-like porous structure transforms into an array of tubes with an F − -rich layer between the TiO 2 layer and the Ti metal. As a result, a hemispherical oxide/metal interfacial structure is formed. The overall growth rate and the length of the nanotubes are determined by the difference between the oxide formation and dissolution reaction rates.
The current-time (I-t) behavior measured during the potentiostatic preparation of TiO 2 nanotubes reflects this overall mechanism ( Figure 2). In the initial stage, the current decreases rapidly due to the increasing resistance of the rapidly growing oxide layer (I). In the second step (II), the current increases slightly due to the formation of nano-sized pits, which are formed due to attack by the F − ions. The local electric fields are strengthened in these pits, thus attracting more anions to participate in the oxide formation and dissolution reactions. As a tubular structure begins to form beneath the pits, the current decreases again (III). When the oxide formation and dissolution reactions reach equilibrium, the current converges (IV). The current-time transient itself cannot confirm the formation of nano-tubular structures, since non-nanotube-forming processes based on the barrier oxide formation, oxide pitting, and the stable growth mechanism show similar current patterns [11]. (I) The current decreases drastically due to the growth of the barrier oxide during initial stage of anodization. Next, (II) nano-pits or cracks caused by F − ions cause an increase in the current due to the concentrated electric fields on these pits. Once the tubular structure has formed and is growing evenly, the current declines and converges at a stable value due to the increased diffusion length of the ions involved in the reaction. Reproduced with permission from ref [11]. Friedrich-Alexander-Universität Erlangen-Nürnberg (2013).

Reaction Parameters
TiO2 nanotubes can be obtained in electrolytes containing halides (ClO4 − , Br − , Cl − , F − ), regardless of the electrolyte solvent. The use of F − salts is favorable to prepare uniformly oriented TiO2 nanotube arrays [31,44,45]. When Cl − or Br − are added to the electrolyte, non-uniform bundle-like nanotubular structures are easily generated; this is known as rapid breakdown anodization (RBA) [30,[44][45][46]. Generally, 0.05-2% F − ion is considered to be appropriate for the formation of TiO2 nanotubes [11,31]. After selecting the F − concentration, the environment of the electrolyte is determined depending on the type of solvent. HF is a typical F − source that is widely utilized in aqueous conditions. Additionally, it is recommended to adjusting the pH of electrolyte to neutrality; sulfuric acid, phosphoric acid, and acetic acid are typical acids used for this purpose, and NaOH or KOH are generally used as bases. Shifting the pH of the solution into the weakly acidic range results in longer nanotubes [47][48][49]. Feasible anodization voltages range from 5 to 30 V in aqueous conditions [11].
Ethylene glycol and glycerol are the most commonly used organic solvents for TiO2 nanotube growth. The use of ethylene glycol is favored due to the low glycerol solubility of F − containing salts such as NH4F, which are widely used as the F − source [50,51]. When these solvents are used, the electrolyte is normally weakly basic, demonstrating that basic conditions can also be used to prepare TiO2 nanotubes. However, water is an essential component for the generation of TiO2. For this reason, 1-10% of water is usually added directly to the organic electrolyte [8,11,16,31,43]. TiO2 nanotubes can be prepared over a very wide range of applied voltages in ethylene glycol; they are easily and uniformly grown via potentiostatic methods without any additional control technique in the range 25-100 V [31,52]. The recently reported ramping method is a powerful solution to avoid the breakdown of the oxide and to form nanotubes evenly at voltages above 100 V under organic conditions [52,53].
The pore size of the TiO2 nanotubes is governed by intensity of the applied voltage. Normally, pores with sizes of 10-100 nm can be produced using the typical voltage ranges given above [11,44,54,55]. For instance, a pore size of around 100 nm is easily obtained at 20 V. Similarly, the size (I) The current decreases drastically due to the growth of the barrier oxide during initial stage of anodization. Next, (II) nano-pits or cracks caused by F − ions cause an increase in the current due to the concentrated electric fields on these pits. Once the tubular structure has formed and is growing eVenly, the current declines and converges at a stable value due to the increased diffusion length of the ions involved in the reaction. Reproduced with permission from ref [11]. Friedrich-Alexander-Universität Erlangen-Nürnberg (2013). regardless of the electrolyte solvent. The use of F − salts is favorable to prepare uniformly oriented TiO 2 nanotube arrays [31,44,45]. When Cl − or Br − are added to the electrolyte, non-uniform bundle-like nanotubular structures are easily generated; this is known as rapid breakdown anodization (RBA) [30,[44][45][46]. Generally, 0.05-2% F − ion is considered to be appropriate for the formation of TiO 2 nanotubes [11,31]. After selecting the F − concentration, the environment of the electrolyte is determined depending on the type of solvent. HF is a typical F − source that is widely utilized in aqueous conditions. Additionally, it is recommended to adjusting the pH of electrolyte to neutrality; sulfuric acid, phosphoric acid, and acetic acid are typical acids used for this purpose, and NaOH or KOH are generally used as bases. Shifting the pH of the solution into the weakly acidic range results in longer nanotubes [47][48][49]. Feasible anodization voltages range from 5 to 30 V in aqueous conditions [11]. Ethylene glycol and glycerol are the most commonly used organic solvents for TiO 2 nanotube growth. The use of ethylene glycol is favored due to the low glycerol solubility of F − containing salts such as NH 4 F, which are widely used as the F − source [50,51]. When these solvents are used, the electrolyte is normally weakly basic, demonstrating that basic conditions can also be used to prepare TiO 2 nanotubes. However, water is an essential component for the generation of TiO 2 . For this reason, 1-10% of water is usually added directly to the organic electrolyte [8,11,16,31,43]. TiO 2 nanotubes can be prepared over a very wide range of applied voltages in ethylene glycol; they are easily and uniformly grown via potentiostatic methods without any additional control technique in the range 25-100 V [31,52]. The recently reported ramping method is a powerful solution to avoid the breakdown of the oxide and to form nanotubes eVenly at voltages above 100 V under organic conditions [52,53].

Reaction Parameters
The pore size of the TiO 2 nanotubes is governed by intensity of the applied voltage. Normally, pores with sizes of 10-100 nm can be produced using the typical voltage ranges given above [11,44,54,55]. For instance, a pore size of around 100 nm is easily obtained at 20 V. Similarly, the size of the pores produced in ethylene glycol solution is proportional to the applied voltage, but a voltage of 40-45 V corresponds to a pore size of 100 nm [31,56,57].
Moreover, it has been reported that the pore size can be expanded to 600 nm or more using the ramping technique, similarly to in the anodization of aluminum [52,53].
If the oxide formation rate is faster than the oxide dissolution rate, the length of the TiO 2 nanotubes will increase as a function of anodization time. When the rates of these two competitive reactions are in a steady-state equilibrium, the growth of nanotubes is halted, and they maintain their length. In general, TiO 2 nanotubes prepared in an organic electrolyte are much longer than those prepared in aqueous solution. The longest reported nanotubes produced under aqueous conditions were of 7.3 µm in length, but 1-3 µm nanotubes are achieved in most cases [11,31,49,58,59]. In contrast, nanotubes tens or hundreds of µm in length can be grown in ethylene glycol, allowing researchers to adjust the length of the nanotubes from a few hundreds of nanometers to micrometers by controlling the anodization time [8,31,56,57]. However, longer anodization time causes the formation of nanograsses, which are produced by nanotubes splitting in the direction of the applied electric field of the F − ions. Since the nanograss blocks the movement of ions into the pores, several methods for its removal have been developed [13,59].

Doping of TiO 2 Nanotubes
As mentioned earlier, TiO 2 nanotubes provide an enormous electrochemical reaction surface area due to their high aspect-ratio. For example, TiO 2 nanotubes with a pore diameter of 100 nm and the aspect-ratio of 10 provide a surface area that is 120 times higher (0.785 cm 2 → 94.2 cm 2 ) than that of a flat TiO 2 surface [31]. Nonetheless, suitable catalysts or active materials must be used to overcome the insulating properties of TiO 2 . In this section, we discuss methods of doping TiO 2 nanotubes.

Single-Step Anodization
Single-step anodization is a doping method based on the principle of plastic flow. The salt of an anion complex containing the target metal oxide is selected as the precursor. This salt is added directly to the conventional electrolyte to prepare the nanotubes. As shown in Figure 3a, nanotubes will not be produced if the electrolyte is not suitable for the typical anodic conditions used to produce nanotubular structures [17,24,31,47]. In addition, an electrolyte is difficult to be used if the precursor is vulnerable to F − ion [34].
The doping mechanism is almost the same as the anodization mechanism. The precursor anion participates in the two main reaction processes of oxide formation and dissolution. If the target dopant is Ru or Ir oxide, which are widely used for water oxidation catalysts, the catalyst doped into the nanotubes can be partially dissolved via the oxygen eVolution reaction during prolonged anodization [17,24,31]. As a result, the doping concentration of the catalyst at the growth site will be much higher than that of the sidewalls of the nanotubes (Figure 3b).
Yoo et al. successfully doped RuO 2 into TiO 2 nanotubes via single-step anodization in an ethylene-glycol-based electrolyte containing 0.25% NH 4 F and 5% water. RuO 2 -doped TiO 2 nanotubes with a doping concentration of 0.12 at.% were produced in the same anodizing electrolyte with the addition of 0.02 M KRuO 4 . The RuO 2 -doped TiO 2 nanotubes prepared at 40 V for 22 h were approximately 30% longer than conventional nanotubes prepared without KRuO 4 [17]. The doping concentration increased to 1.21 at.% when an aqueous medium was used due to the effect of water. During the synthesis of the nanotubes, the precursor KRuO 4 is dissociated into K + and RuO 4 − , the latter of which takes part in the following relevant reactions: Figure 3. (a) A schematic of the conventional anodization procedure and doping methods. Note that potential shock is a sequential two-step anodic process. (b) Left: The doping of the catalysts follows "plastic flow." The doped catalysts are able to partially dissolve at long doping times, as the high anodic potential induces the oxygen evolution reaction. Right: The morphologies of the doped TiO2 nanotubes depends on the doping method. Reproduced with permission from ref [31]. Inha University (2018). (4) and (5), both RuO2 and TiO2 are formed from RuO4 − simultaneously. As a result, the wall thickness of the nanotubes increased, as shown in Figure 4. The wall thickness of the nanotubes increases from 5.73 nm to 13.96 nm in the presence of the catalyst precursor of KRuO4. The thickness can be further increased (13.96 nm → 25.74 nm) when electrolyte contains small amount of water, which can be explained by simultaneous formation of TiO2 and RuO2 in Equations (4) and (5). The rutile RuO2 phase determined by SAED analysis provides a clear evidence for doping ( Figure 4d).

As shown in Equations
Furthermore, simultaneous co-doping of TiO2 nanotubes with IrO2 and RuO2 can be achieved by single-step anodization using the electrolyte 1 M H3PO4 + 1 M NaOH + 0.3-0.7 vol.% HF containing KRuO4 and IrOx nanoparticles, which are prepared as an intermediate species for IrO2 doping. Since chloride ions, which damage the NTs, are typically involved in Ir precursors, IrOx nanoparticles are used to generate IrO4 − in the electrolyte along with the RuO4 − for RuO2 doping [24].

As shown in Equations
As a result, the wall thickness of the nanotubes increased, as shown in Figure 4. The wall thickness of the nanotubes increases from 5.73 nm to 13.96 nm in the presence of the catalyst precursor of KRuO 4 . The thickness can be further increased (13.96 nm → 25.74 nm) when electrolyte contains small amount of water, which can be explained by simultaneous formation of TiO 2 and RuO 2 in Equations (4) and (5). The rutile RuO 2 phase determined by SAED analysis provides a clear eVidence for doping ( Figure 4d). Furthermore, simultaneous co-doping of TiO 2 nanotubes with IrO 2 and RuO 2 can be achieved by single-step anodization using the electrolyte 1 M H 3 PO 4 + 1 M NaOH + 0.3-0.7 vol.% HF containing KRuO 4 and IrO x nanoparticles, which are prepared as an intermediate species for IrO 2 doping. Since chloride ions, which damage the NTs, are typically involved in Ir precursors, IrO x nanoparticles are used to generate IrO 4 − in the electrolyte along with the RuO 4 − for RuO 2 doping [24].
Therefore, the overall morphology of co-doped TiO 2 is similar to that of TiO 2 nanotubes singly doped with RuO 2 . Under the optimized conditions, the doping concentration of IrO 2 in the TiO 2 layer of binary-catalyst-doped TiO 2 is usually about half that of RuO 2 , exhibiting polycrystalline after annealing.
Tin oxide is also frequently used as a dopant to control the bandgap and overpotential of TiO 2 . Unlike the doping precursors discussed above, tin oxide, which can be easily obtained from Na 2 SnO 3 , is used at basic pH; basic conditions are not typically used for the anodization of Ti in aqueous conditions. Ma  Tin oxide is also frequently used as a dopant to control the bandgap and overpotential of TiO2. Unlike the doping precursors discussed above, tin oxide, which can be easily obtained from Na2SnO3, is used at basic pH; basic conditions are not typically used for the anodization of Ti in aqueous conditions. Ma et al. reported that an ethylene glycol-based electrolyte containing both Na2SnO3 and Na2MoO4 · 4H2O led to the formation of TiO2 nanotubes containing both 0.28% MoO3 (Mo 6+ ) and 0.51 at.% SnO2 (Sn 4+ ) [60]. Very recently, we reported that WO3 can also be doped onto TiO2 nanotubes using a phosphoricacid-based aqueous electrolyte containing Na2WO4. The doping concentration increased linearly with the concentration of the precursor. The WO3-doped TiO2 nanotubes showed 17% higher electrochromic performance than bare TiO2 nanotubes at the optimum doping concentration of 0.21 at.% [47].

Anodic Potential Shock
The anodic potential shock method was first reported by Jo et al. in 2009 [61]. Originally, it was designed for the preparation of through-hole type TiO2 membranes. The same group later adopted this method to introduce dopants in/on anodic structures through modification of the anodization parameters [32,62,63]. This method is regarded as a two-step anodization, with each step being performed in a different electrolyte. In the first step, the formation of nanotubes takes place. In the second step, an extremely high anodic voltage is applied to the prepared nanotubes for a very short period ( Figure 1a); the doping precursor is only present in the electrolyte used during the second step. The precursors used are almost the same as those in the single-step anodization, but the oxide formation and doping reactions are independent. Therefore, the oxide formation follows the anodization mechanism exactly (see Figure 1b), and the doping results from high-field migration under a sudden high potential.
We showed that RuO2 could be doped into TiO2 barrier structure via the potential shock method using KRuO4 as the precursor [63]. The average doping concentration of Ru in TiO2 at a shock voltage of 140 V was over 4 at.%. The two-step anodic doping method resulted in a much higher Ru concentration at the base of the nanotubes than in the walls, similarly to in single-step anodization [31,32]. However, additional barrier oxide was formed at the bottom of the tubes due to the absence of Fions in the doping electrolyte; its thickness was a function of the applied potential shock voltage (see Figure 5). Using a similar method, Seong et al. succeeded in producing TiO2 nanotubes with 0.7 Very recently, we reported that WO 3 can also be doped onto TiO 2 nanotubes using a phosphoric-acid-based aqueous electrolyte containing Na 2 WO 4 . The doping concentration increased linearly with the concentration of the precursor. The WO 3 -doped TiO 2 nanotubes showed 17% higher electrochromic performance than bare TiO 2 nanotubes at the optimum doping concentration of 0.21 at.% [47].

Anodic Potential Shock
The anodic potential shock method was first reported by Jo et al. in 2009 [61]. Originally, it was designed for the preparation of through-hole type TiO 2 membranes. The same group later adopted this method to introduce dopants in/on anodic structures through modification of the anodization parameters [32,62,63]. This method is regarded as a two-step anodization, with each step being performed in a different electrolyte. In the first step, the formation of nanotubes takes place. In the second step, an extremely high anodic voltage is applied to the prepared nanotubes for a very short period (Figure 1a); the doping precursor is only present in the electrolyte used during the second step. The precursors used are almost the same as those in the single-step anodization, but the oxide formation and doping reactions are independent. Therefore, the oxide formation follows the anodization mechanism exactly (see Figure 1b), and the doping results from high-field migration under a sudden high potential.
We showed that RuO 2 could be doped into TiO 2 barrier structure via the potential shock method using KRuO 4 as the precursor [63]. The average doping concentration of Ru in TiO 2 at a shock voltage of 140 V was over 4 at.%. The two-step anodic doping method resulted in a much higher Ru concentration at the base of the nanotubes than in the walls, similarly to in single-step anodization [31,32]. However, additional barrier oxide was formed at the bottom of the tubes due to the absence of Fions in the doping electrolyte; its thickness was a function of the applied potential shock voltage (see Figure 5). Using a similar method, Seong et al. succeeded in producing TiO 2 nanotubes with 0.7 at.% MnO 2 from the precursor KMnO 4 in ethylene glycol media; the nanotubes showed enhanced water oxidation performance under alkaline conditions [34]. at.% MnO2 from the precursor KMnO4 in ethylene glycol media; the nanotubes showed enhanced water oxidation performance under alkaline conditions [34]. For Pt doping, Cl − -based complexes such as H2PtCl6 are typically available as reaction-grade chemicals. Kim et al. prepared TiO2 nanotubes doped with 3 ppm of PtO for application in the hydrogen evolution reaction. In this case, a shock voltage below 20 V was utilized because higher voltages (over 20 V) caused the collapse of the tubular arrays via attack by the Cl − ions. Since the applied potential shock voltage was far lower than the anodization voltage, this method is referred to as the underpotential shock method [33].
It is possible to use the potential shock method with any metal oxide catalyst, as long as the precursor is sufficiently soluble in a suitable solvent. However, the entrances to the pores must remain clear to allow the precursors easy access to the deep sites of the nanotubes. For this reason, TiO2 nanotubes prepared in aqueous solution are much preferred. However, the possibility of using potential shock under other conditions has been suggested, as techniques to remove the nanograss that gradually develops during anodization have been reported [64][65][66].

Doping via Thermal Treatment
Anodically formed TiO2 nanotube layers are normally amorphous [67,68]; however, when anodization is carried under specific conditions at higher voltages, nanocrystallites are present [35,67,69]. However, for use in many applications, the amorphous tubes must be crystallized by thermal treatment. In general, amorphous nanotubes can be converted to the anatase or rutile phases by thermal treatment at 300-500 °C or 550 °C, respectively. The bandgap energy of a crystallized TiO2 nanotube is 3.2 eV after conversion to anatase, and 3.0 eV after conversion to rutile [68]. For certain applications, such as solar cells and photocatalysis, the bandgap energy of these structures is too wide. To enhance their efficiency in such applications, the bandgap energy must be tuned. The most wellknown approach for adjusting the bandgap is to dope metal or non-metal impurities into the TiO2 nanotubes.
Asahi et al. reported that nitrogen-doping of TiO2 enhanced its visible photoresponse. Their report demonstrated that the doped nitrogen, which substituted for the oxygen of TiO2, narrowed the bandgap energy by introducing N2p states just above the valence band of TiO2 [15]. The classic approach to oxygen-substitution-doping of TiO2 nanotubes involves ion implantation [26,27,[70][71][72]. This method is most effective at introducing nitrogen into the TiO2 lattice at low-to-medium doping levels (about 10 18 ions/cm 2 ) [26,27]. However, this method has several shortcomings: the ion penetration depth is limited to a few micrometers, a relatively high acceleration energy of several MeV is required, and the distribution of the dopant in the TiO2 structure is often inhomogeneous. Moreover, after implantation, amorphization of the TiO2 nanotubes occurs, making a reannealing process to reestablish the crystalline structure necessary. A simpler approach for doping nitrogen into TiO2 is thermal treatment in NH3 [70]. Such thermal treatments are generally performed in a NH3/Ar atmosphere at relatively high temperatures (above 500 °C) [29]. For Pt doping, Cl − -based complexes such as H 2 PtCl 6 are typically available as reaction-grade chemicals. Kim et al. prepared TiO 2 nanotubes doped with 3 ppm of PtO for application in the hydrogen eVolution reaction. In this case, a shock voltage below 20 V was utilized because higher voltages (over 20 V) caused the collapse of the tubular arrays via attack by the Cl − ions. Since the applied potential shock voltage was far lower than the anodization voltage, this method is referred to as the underpotential shock method [33].
It is possible to use the potential shock method with any metal oxide catalyst, as long as the precursor is sufficiently soluble in a suitable solvent. However, the entrances to the pores must remain clear to allow the precursors easy access to the deep sites of the nanotubes. For this reason, TiO 2 nanotubes prepared in aqueous solution are much preferred. However, the possibility of using potential shock under other conditions has been suggested, as techniques to remove the nanograss that gradually develops during anodization have been reported [64][65][66].

Doping via Thermal Treatment
Anodically formed TiO 2 nanotube layers are normally amorphous [67,68]; however, when anodization is carried under specific conditions at higher voltages, nanocrystallites are present [35,67,69]. However, for use in many applications, the amorphous tubes must be crystallized by thermal treatment. In general, amorphous nanotubes can be converted to the anatase or rutile phases by thermal treatment at 300-500 • C or 550 • C, respectively. The bandgap energy of a crystallized TiO 2 nanotube is 3.2 eV after conversion to anatase, and 3.0 eV after conversion to rutile [68]. For certain applications, such as solar cells and photocatalysis, the bandgap energy of these structures is too wide. To enhance their efficiency in such applications, the bandgap energy must be tuned. The most well-known approach for adjusting the bandgap is to dope metal or non-metal impurities into the TiO 2 nanotubes.
Asahi et al. reported that nitrogen-doping of TiO 2 enhanced its visible photoresponse. Their report demonstrated that the doped nitrogen, which substituted for the oxygen of TiO 2 , narrowed the bandgap energy by introducing N2p states just above the valence band of TiO 2 [15]. The classic approach to oxygen-substitution-doping of TiO 2 nanotubes involves ion implantation [26,27,[70][71][72]. This method is most effective at introducing nitrogen into the TiO 2 lattice at low-to-medium doping levels (about 10 18 ions/cm 2 ) [26,27]. However, this method has several shortcomings: the ion penetration depth is limited to a few micrometers, a relatively high acceleration energy of several MeV is required, and the distribution of the dopant in the TiO 2 structure is often inhomogeneous. Moreover, after implantation, amorphization of the TiO 2 nanotubes occurs, making a reannealing process to reestablish the crystalline structure necessary. A simpler approach for doping nitrogen into TiO 2 is thermal treatment in NH 3 [70]. Such thermal treatments are generally performed in a NH 3 /Ar atmosphere at relatively high temperatures (above 500 • C) [29].
Based on the peak position of nitrogen observed from sputtering TiO 2 under nitrogen atmosphere and titanium nitride [29], successful nitrogen doping should result in a nitrogen (N1s) peak located at~396 eV in XPS analysis [28,29,72]. However, in some reports, this nitrogen peak was observed at~400 eV or above 400 eV [73][74][75]. These higher peak values correspond to surface adsorption or sensitization of nitrogen on the TiO 2 surface as N-C compounds or molecular N 2 [76]. Several research groups have claimed to have successfully doped nitrogen into TiO 2 via solution-based doping. Other reports eVen claim that the nitrogen doping concentration in TiO 2 is increased by prolonged anodization. However, these results require further confirmation, as they resulted in N peaks located at~400 eV [73][74][75][76]. Moreover, most of these reports did not show suitable eVidence of bandgap engineering via visible photocurrent spectra or visible photocatalytic activity.
Carbon has also been suggested as a dopant to form states near the valence band by the substitution of oxygen [25,77,78]. Furthermore, carbon doping can also be achieved by the thermal treatment of TiO 2 in a carbonaceous environment or ashing organic compounds, such as CO or acetylene [79][80][81]. The thermal doping of carbon should be carefully defined to differentiate it from graphitization or the formation of oxy-carbides of the TiO 2 nanotubes [82,83]. The thermal treatment of TiO 2 nanotubes in an acetylene environmental can also convert them to TiO x C y materials with semimetallic conductivity comparable to that of graphite [83]. Solution-based carbon doping is also frequently attempted. However, these results cannot consider carbon residue from decomposition of the organic electrolyte. The organic solvent in the anodization electrolyte can be decomposed by the applied high potential and remain inside the nanotube wall [67,84].

Alloy-Based Anodization
The simplest and most straightforward doping approach is the anodization of alloys that contain the dopant material. Using this method, nitrogen-doped TiO 2 nanotubes can be obtained by the anodization of TiN substrates [85,86], which can be prepared by arc-melting Ti and TiN powders. A similar approach involves anodizing Ti-transition metal alloys to produce metal-or metal-oxide-doped TiO 2 nanotubes [87][88][89]. Density functional theory (DFT) calculations have shown that various transition metals are effective dopants for Ti substitution in TiO 2 structures to form intermediate states in the bandgap [90]. The substitution of Ti by such dopants leads to a red-shift in the optical properties of the nanotubes [91][92][93][94], enhancing its electrical conductivity [95][96][97][98]. Metal oxides can also substitute Ti, as in the example of W doping. When tungsten is doped at Ti sites, it forms WO 3 in the TiO 2 lattice. Each W 6+ associates with an extra oxygen instead of Ti 4+ . The WO 3 -doped TiO 2 has a narrower bandgap as a result of its lower conduction band [99].
When preparing metal-or metal-oxide-doped TiO 2 nanotubes by the anodization of a Ti alloy, the dopant materials must not interfere with the anodic reaction. That is, in order to successfully prepare porous or tubular structures, only a very small amount of the dopant materials should be present in the Ti alloy, and the dopant materials should have chemical properties similar to those of Ti. If the chemical properties of the dopant are too different from those of Ti, or if too much dopant is present in the Ti alloy, the resulting nanotube structures may be irregular, or in the worst case, only a compact oxide will be formed ( Figure 6).
In many cases, interesting morphology such as two-scaled nanotube structures (two length scales or two distinct tube diameters) are formed during the anodization of certain alloys [100][101][102][103][104]. Such morphologies may be caused by the different oxidation or dissolution kinetics of Ti and the dopant metals, but the phenomena are still not completely understood [105][106][107]. The metal composition of the anodic oxide formed from a Ti alloy depends on the metal ratio in the alloy substrate [108]. In some cases, small amounts of mixed oxides may be present in the anodic oxide structures. So far, complete mixed oxide conversion has only been reported for TiZr alloys [109].
Earlier studies of doped TiO 2 nanotubes prepared by the anodization of alloys focused on enhancing ion insertion to improve their electrochromic properties [87][88][89]110,111]. In particular, WO 3 , MO 3 , and Nb 2 O 5 -doped TiO 2 nanotubes formed by the anodization of Ti-W, Ti-Mo, and Ti-Nb alloys showed significantly improved electrochromic efficiency and ion (particularly, H + ) insertion properties when eVen a small amount of dopant (0.2 at.% of WO 3 ) was present [87,88,[110][111][112][113]. Moreover, TiO 2 -Nb 2 O 5 mixed-oxide nanotubes showed high ion intercalation stability and electrochromic activity. These results were due to the widening of the TiO 2 lattice by Nb ions, which was observed using high-resolution transmission electron microscopy (HRTEM) analysis and predicted by DFT calculations [88]. The lattice-widened TiO 2 nanotubes allow lager guest ions such as Li + and Na + to intercalate into the lattice, as well as making the H + intercalation process faster [88]. Moreover, TiO2-Nb2O5 mixed-oxide nanotubes showed high ion intercalation stability and electrochromic activity. These results were due to the widening of the TiO2 lattice by Nb ions, which was observed using high-resolution transmission electron microscopy (HRTEM) analysis and predicted by DFT calculations [88]. The lattice-widened TiO2 nanotubes allow lager guest ions such as Li + and Na + to intercalate into the lattice, as well as making the H + intercalation process faster [88]. Obviously, the anodic oxidation of Ti alloys in F − -containing electrolytes allows a wide range of dopants to be effectively doped into TiO2 nanotubes. Moreover, the doped TiO2 nanotubes formed from Ti alloys provide virtually unlimited potential to enhance the chemical and physical properties of the TiO2 nanotubes. Specific examples of such enhancements will be discussed in the applications section.

Electrochemical Water Electrolysis
The electrochemical oxygen evolution reaction (OER) is a four-electron transfer reaction consisting of four single electron transfer reactions. Therefore, the use of catalysts is essential to reduce the overpotential, which is driven by the multiple electron transfer steps [115][116][117]. Increasing the amount of oxygen evolution at a given overpotential is becoming an important research topic [115,118]. A high reaction surface area is an important factor in producing a large amount of oxygen gas. Moreover, a durable support material is required, because the electrode is continuously exposed to corrosive oxygen radicals [119,120]. Thus, TiO2 nanotubes, which have inherent anti-corrosive properties, are expected to be a good electrode material for this application. Decorating or doping catalysts onto/into high-aspect-ratio TiO2 nanotubes is difficult, as the mouths of nanotubes can become blocked by precipitated catalyst if improper methods are employed. However, the problem of pore loss can be effectively solved by preparing the catalyst-assisted TiO2 via the doping methods described in the previous sections. Obviously, the anodic oxidation of Ti alloys in F − -containing electrolytes allows a wide range of dopants to be effectively doped into TiO 2 nanotubes. Moreover, the doped TiO 2 nanotubes formed from Ti alloys provide virtually unlimited potential to enhance the chemical and physical properties of the TiO 2 nanotubes. Specific examples of such enhancements will be discussed in the applications section.

Electrochemical Water Electrolysis
The electrochemical oxygen eVolution reaction (OER) is a four-electron transfer reaction consisting of four single electron transfer reactions. Therefore, the use of catalysts is essential to reduce the overpotential, which is driven by the multiple electron transfer steps [115][116][117]. Increasing the amount of oxygen eVolution at a given overpotential is becoming an important research topic [115,118]. A high reaction surface area is an important factor in producing a large amount of oxygen gas. Moreover, a durable support material is required, because the electrode is continuously exposed to corrosive oxygen radicals [119,120]. Thus, TiO 2 nanotubes, which have inherent anti-corrosive properties, are expected to be a good electrode material for this application. Decorating or doping catalysts onto/into high-aspect-ratio TiO 2 nanotubes is difficult, as the mouths of nanotubes can become blocked by precipitated catalyst if improper methods are employed. However, the problem of pore loss can be effectively solved by preparing the catalyst-assisted TiO 2 via the doping methods described in the previous sections. TiO 2 nanotubes that are singly doped with RuO 2 via single-step anodization exhibit overpotentials in the range of 770-1000 mV [17,31,32,121]. The ideal Tafel plot slopes for the first, second, and third electron transfer steps in the OER mechanism have been reported to be 120, 40, and 30 mV/dec, meaning that the slope of Tafel should be lower than these values to achieve an excellent electron transfer rate. The Tafel slopes of nanotubes produced by single-step anodization are in the range of 37-46 mV/dec, indicating that the rate-determining step (RDS) for the OER in the nanotubes is located near the second electron transfer step. Nanotubes doped with RuO 2 using the potential shock method exhibit a lower overpotential (650 mV) than those produced via single-step anodization. However, the RDS when using these nanotubes for the OER has been reported to be the second electron transfer step, as they have a Tafel slope of 46 mV/dec [31,[122][123][124].
The slow electron transfer of electrodes produced via the potential shock method can be explained in terms of morphological changes; the increased thickness of the barrier oxide at the bottom of the tubes increases the electron transfer resistance [31,54]. However, despite the thick barrier oxide, the overpotential of nanotubes prepared by the potential shock is lower than that of those prepared by single-step anodization. This is due to the surface chemical composition of the catalysts. Ru-O bonding, which effectively diminishes the overpotential, is dominant on the surface of the potential shock nanotubes [125][126][127]. On the other hand, Ru-OH, which increases the overpotential, is dominant on the surface of the single-step anodization nanotubes [31,121].
A complex variety of factors determine the current density in the OER. Increased surface area and an increased doping concentration of Ru in TiO 2 lead to higher current density, whereas increased barrier layer thickness reduces the current density ( Figure 7). Overall, based on empirical experimental data from RuO 2 -doped TiO 2 nanotubes, we found that the OER current is determined by three major factors according to the following relationship: TiO2 nanotubes that are singly doped with RuO2 via single-step anodization exhibit overpotentials in the range of 770-1000 mV [17,31,32,121]. The ideal Tafel plot slopes for the first, second, and third electron transfer steps in the OER mechanism have been reported to be 120, 40, and 30 mV/dec, meaning that the slope of Tafel should be lower than these values to achieve an excellent electron transfer rate. The Tafel slopes of nanotubes produced by single-step anodization are in the range of 37-46 mV/dec, indicating that the rate-determining step (RDS) for the OER in the nanotubes is located near the second electron transfer step. Nanotubes doped with RuO2 using the potential shock method exhibit a lower overpotential (650 mV) than those produced via single-step anodization. However, the RDS when using these nanotubes for the OER has been reported to be the second electron transfer step, as they have a Tafel slope of 46 mV/dec [31,[122][123][124].
The slow electron transfer of electrodes produced via the potential shock method can be explained in terms of morphological changes; the increased thickness of the barrier oxide at the bottom of the tubes increases the electron transfer resistance [31,54]. However, despite the thick barrier oxide, the overpotential of nanotubes prepared by the potential shock is lower than that of those prepared by single-step anodization. This is due to the surface chemical composition of the catalysts. Ru-O bonding, which effectively diminishes the overpotential, is dominant on the surface of the potential shock nanotubes [125][126][127]. On the other hand, Ru-OH, which increases the overpotential, is dominant on the surface of the single-step anodization nanotubes [31,121].
A complex variety of factors determine the current density in the OER. Increased surface area and an increased doping concentration of Ru in TiO2 lead to higher current density, whereas increased barrier layer thickness reduces the current density ( Figure 7). Overall, based on empirical experimental data from RuO2-doped TiO2 nanotubes, we found that the OER current is determined by three major factors according to the following relationship:  . Linear relationship of the alkaline OER current density with the overpotential and the morphological parameters of doping concentration, surface area, and nanotube thickness for RuO2doped TiO2 nanotubes. ①, ②, and ③ correspond to RuO2 doping via single-step anodization in organic solvent, single-step anodization in aqueous conditions, and potential shock in aqueous conditions. Reproduced with permission from reference [31]. Inha University (2018).
TiO2 nanotubes doped with MnO2 via potential shock have been used as an improved non-noble metal catalyst in alkaline OER electrodes [34]. Pt, specifically PtO, which is doped into TiO2 nanotubes Figure 7. Linear relationship of the alkaline OER current density with the overpotential and the morphological parameters of doping concentration, surface area, and nanotube thickness for RuO 2 -doped TiO 2 nanotubes. 1 , 2 , and 3 correspond to RuO 2 doping via single-step anodization in organic solvent, single-step anodization in aqueous conditions, and potential shock in aqueous conditions. Reproduced with permission from reference [31]. Inha University (2018). TiO 2 nanotubes doped with MnO 2 via potential shock have been used as an improved non-noble metal catalyst in alkaline OER electrodes [34]. Pt, specifically PtO, which is doped into TiO 2 nanotubes by underpotential shock, provides enhanced performance in both the OER and HER (hydrogen eVolution reaction) [33]. RuO 2 and IrO 2 co-doping of TiO 2 nanotubes shows a synergetic effect in reducing overpotential. Such co-doped nanotubes exhibited an overpotential of 590 mV with the third electron transfer step [128]. This electrode eVolved twice the amount of oxygen gas compared to a powder-type electrode material with identical components (Figure 8) [24,128,129]. by underpotential shock, provides enhanced performance in both the OER and HER (hydrogen evolution reaction) [33]. RuO2 and IrO2 co-doping of TiO2 nanotubes shows a synergetic effect in reducing overpotential. Such co-doped nanotubes exhibited an overpotential of 590 mV with the third electron transfer step [128]. This electrode evolved twice the amount of oxygen gas compared to a powder-type electrode material with identical components (Figure 8) [24,128,129].

Photocatalysis and Photoelectrochemical Water Splitting
Since the first report of photocatalytic water splitting on TiO2 by Fujishima and Honda in 1972 [130], TiO2 has been considered to be one of the best materials for photocatalysts. It has excellent photooxidative activity for the degradation of organic pollutants, toxins, and bacteria [130][131][132][133][134][135][136]. Two main reactions occur simultaneously in a photocatalytic system: photooxidation from holes on the surface of the valence band edge and photoreduction from the electrons on the surface of conduction bad edge.
Among the various metal-and metal-oxide-doped TiO2 nanotubes, WO3-doped TiO2 nanotubes most effectively increase photocatalytic activity [141]. In contrast to Al-doped nanotubes (one of the most efficient additives for inducing carrier recombination [89,141]), mixed-oxide TiO2 nanotubes doped with both WO3 and MoO3 show strongly enhanced photocatalytic activity compared with nondoped tubes. The highly beneficial effect of W and Mo cannot be explained by better charge transport in the tubes but is instead ascribed to modification of the band or surface state distribution of the doped nanotubes [89,112,141].

Photocatalysis and Photoelectrochemical Water Splitting
Since the first report of photocatalytic water splitting on TiO 2 by Fujishima and Honda in 1972 [130], TiO 2 has been considered to be one of the best materials for photocatalysts. It has excellent photooxidative activity for the degradation of organic pollutants, toxins, and bacteria [130][131][132][133][134][135][136]. Two main reactions occur simultaneously in a photocatalytic system: photooxidation from holes on the surface of the valence band edge and photoreduction from the electrons on the surface of conduction bad edge.
Among the various metal-and metal-oxide-doped TiO 2 nanotubes, WO 3 -doped TiO 2 nanotubes most effectively increase photocatalytic activity [141]. In contrast to Al-doped nanotubes (one of the most efficient additives for inducing carrier recombination [89,141]), mixed-oxide TiO 2 nanotubes doped with both WO 3 and MoO 3 show strongly enhanced photocatalytic activity compared with non-doped tubes. The highly beneficial effect of W and Mo cannot be explained by better charge transport in the tubes but is instead ascribed to modification of the band or surface state distribution of the doped nanotubes [89,112,141].
Photoelectrochemical water splitting is another promising application for anodic TiO 2 nanotubes. Like photocatalysis, the photoelectrochemical water splitting reaction is based on the light-induced electron-hole pair creation [140]. H 2 O can be oxidized by the hole generated on the TiO 2 surface, and hydrogen eVolution occurs at the counter electrode (such as Pt) by attracting an electron from the TiO 2 conduction band. In this context, the electronic properties of TiO 2 are very important, because they determine how efficiently electrons can be transferred along the one-directional path. Hence, a wide range of investigations into the electrical and optical properties of TiO 2 nanotubes have been performed, as described above.
For photoelectrochemical water splitting, very low amounts of metal or metal oxide dopants such as RuO 2 [149], Nb [148,150], and Ta [151] are used. In RuO 2 -doped TiO 2 nanotubes, the RuO 2 is believed to accelerate the O 2 eVolution reaction by catalytic activity [152][153][154]. On the other hand, TiO 2 nanotubes doped with small amounts of transition metal (such as Nb or Ta) show enhanced the electrical conductivity due to their narrower bandgaps, meaning that the electrons can travel efficiently through the TiO 2 layers to the back contact. The long electron lifetime significantly increases the water splitting efficiency [148,151].

Solar Cells
Another highly promising application of TiO 2 nanotubes is energy conversion devices such as dye-sensitized solar cells (DSSCs). In 1991, Grätzel and O'Regan reported the most significant achievement in this field, the first report of fully fabricated solar cell devices (DSSCs) [155]. The solar cells consisted of a nanocrystalline mesoporous TiO 2 thin-film electrode, a Ru−bipyridyl complex, and an iodine redox electrolyte, and showed a conversion efficiency of 11% [156,157].
As illustrated in Figure 9, electrons are excited from the highest occupied molecular orbital (HOMO) to the lowest unoccupied molecular orbital (LUMO) of the sensitized dye on the TiO 2 surface. The excited electrons are injected into the conduction band of the metal oxide on a femto-to picosecond timescale, and the oxidized dye molecules are reduced by the electrolyte redox reaction within nanoseconds. However, the electron transport rate in TiO 2 and the diffusion rate of the electrolyte are quite slow (micro-to milliseconds) (Figure 9a). For this reason, the overall cell efficiency is determined by the electron transport rate and electrolyte diffusion rate [158]. The electron transport rate and electrolyte diffusion rate compete with the recombination rate of the electrons. Generally, the electron transport rate in TiO 2 nanoparticles is considered to be relatively slow due to surface states, defects, and grain boundaries, which act as electron trapping sites and recombination sites [159][160][161][162][163].
In order to overcome the drawbacks of TiO 2 nanoparticles, one-dimensional TiO 2 nanostructures such as nanorods, nanowires, and nanotubes have been considered for use as photoanodes for DSSCs. Among these nanostructures, anodically formed TiO 2 nanotubes have been considered to be one of the most promising approaches to achieve vertically oriented nanostructures that lead to fast electron pathways [164][165][166][167]. However, the overall conversion efficiency of solar cells based on TiO 2 nanotubes is far lower than that of those based on classical nanoparticles. Anodic TiO 2 nanotube structures still have considerable room for improvement. Several approaches to enhance the overall conversion efficiency of DSSCs by modifying the nanotube structures have been considered. For example, the charge collection efficiency of nanotubes can be improved by electronic, surface, or geometric modification, which directly affects the amount of dye absorption. In addition, front-side illuminated cell construction obviously enhances light harvesting. Metal (such as Nb, Ta or Ru) doping enhances the electrical conductivity of TiO2 nanotubes for use in DSSCs [114,168,169]. Doped TiO2 nanotubes have a slower recombination rate than bare TiO2 nanotubes, improving the electron lifetime [114,168,169]. This beneficial effect has been demonstrated using intensity modulated photovoltage spectroscopy (IMVS), photocurrent spectroscopy (IMPS) measurements, and classical electrochemical impedance spectroscopy [114,168,169] (Figure 10). As a result, the overall conversion efficiency of doped TiO2 nanotubes can be increased by 15-35% compared to non-doped TiO2 nanotubes [114,168,169]. Interestingly, these positive effects vanish in nanostructures with high concentrations of the metal dopants. Metal (such as Nb, Ta or Ru) doping enhances the electrical conductivity of TiO 2 nanotubes for use in DSSCs [114,168,169]. Doped TiO 2 nanotubes have a slower recombination rate than bare TiO 2 nanotubes, improving the electron lifetime [114,168,169]. This beneficial effect has been demonstrated using intensity modulated photovoltage spectroscopy (IMVS), photocurrent spectroscopy (IMPS) measurements, and classical electrochemical impedance spectroscopy [114,168,169] (Figure 10). As a result, the overall conversion efficiency of doped TiO 2 nanotubes can be increased by 15-35% compared to non-doped TiO 2 nanotubes [114,168,169]. Interestingly, these positive effects vanish in nanostructures with high concentrations of the metal dopants. Reproduced with permission from ref [168]. Royal Society of Chemistry (2010) and reference [114]. WILEY-VCH Verlag GmbH and Co. KGaA, Weinheim (2012).

Summary
This paper reviewed the growth of catalyst-doped anodic TiO2 nanotubes and their applications as binder-free electrodes for highly desirable (photo)electrochemical reactions that require a low overvoltage or bandgap. A broad overview of techniques for doping the target materials into anodic TiO2 nanotubes is given.
Concerning the growth of anodic TiO2 nanotubes, we addressed the mechanisms of the reactions that occur during the anodization process and the reaction parameters that influence the structural morphologies of the tubes. The formation of anodic TiO2 nanotubes is guided by oxide formation and dissolution at the interface between the oxide and metal substrate based on a "plastic flow model". In general, electrolytes containing halide ions are suitable for the preparation of TiO2 nanotubes; in particular, electrolytes containing 0.02-2% F − ions are widely used with a constant voltage of 5-30 V in aqueous conditions or 25-100 V in organic conditions. Several techniques for doping foreign elements into high-aspect-ratio TiO2 nanotubes to improve their catalytic properties have also been reviewed in detail. In single-step anodization, a salt  [168]. Royal Society of Chemistry (2010) and reference [114]. WILEY-VCH Verlag GmbH and Co. KGaA, Weinheim (2012).

Summary
This paper reviewed the growth of catalyst-doped anodic TiO 2 nanotubes and their applications as binder-free electrodes for highly desirable (photo)electrochemical reactions that require a low overvoltage or bandgap. A broad overview of techniques for doping the target materials into anodic TiO 2 nanotubes is given.
Concerning the growth of anodic TiO 2 nanotubes, we addressed the mechanisms of the reactions that occur during the anodization process and the reaction parameters that influence the structural morphologies of the tubes. The formation of anodic TiO 2 nanotubes is guided by oxide formation and dissolution at the interface between the oxide and metal substrate based on a "plastic flow model". In general, electrolytes containing halide ions are suitable for the preparation of TiO 2 nanotubes; in particular, electrolytes containing 0.02-2% F − ions are widely used with a constant voltage of 5-30 V in aqueous conditions or 25-100 V in organic conditions. Several techniques for doping foreign elements into high-aspect-ratio TiO 2 nanotubes to improve their catalytic properties have also been reviewed in detail. In single-step anodization, a salt of the anion complex containing the target metal oxide is used as the doping precursor, and is added directly to the electrolyte used for the formation of TiO 2 nanotubes under conventional voltage conditions. As the negatively charged precursor is incorporated into the anodic oxide during anodization, the growth of TiO 2 nanotubes and doping with the target element occur simultaneously. In the anodic potential shock method, the formation of the TiO 2 nanotubes and doping with the target element are performed independently in different electrolytes. After the TiO 2 nanotubes are fabricated, the electrolyte is replaced with an electrolyte containing the anion complex precursor and a potential higher than that of first anodization potential is applied for a short time, which leads to the doping of the negatively charged materials into the anodic oxide.
In addition to electrochemical doping methods, simple and straightforward doping approaches, such as the thermal annealing of TiO 2 nanotubes under a suitable environment or the anodization of an alloy containing the dopant materials can be employed.
Catalyst-doped anodic TiO 2 nanotubes lead to low overpotentials, which are favorable for initiating reactions. For this reason, they are considered to be promising electrodes for electrochemical applications. The overpotential for electrochemical water electrolysis can be reduced to 650 mV via doping of TiO 2 nanotubes. Due to the morphological changes and surface composition of the catalyst on the electrode surface, it is difficult to further reduce the overvoltage for OER.
In addition, metal or metal oxide (Nb, Ta, Ru, WO 3 or MoO 3 )-doped TiO 2 nanotubes show superior photocatalytic and photoelectrochemical water splitting performance compared to non-doped TiO 2 nanotubes due to bandgap engineering and their surface state distribution. Nb, Ta, or Ru-doped TiO 2 nanotubes show higher overall conversion efficiency in DSSCs as a result of their slower recombination rate and enhanced electron lifetime.